Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

PAPER

Cite this: Phys. Chem. Chem. Phys., 2015, 17, 11670

View Journal | View Issue

Assessing thermochemical properties of materials through ab initio quantum-mechanical methods: the case of a-Al2O3 Alessandro Erba,*a Jeﬀerson Maul,ab Raﬀaella Demichelisc and Roberto Dovesia The thermochemical behavior of a-Al2O3 corundum in the whole temperature range 0–2317 K (melting point) and under pressures up to 12 GPa is predicted by applying ab initio methods based on the density functional theory (DFT), the use of a local basis set and periodic-boundary conditions. Thermodynamic properties are treated both within and beyond the harmonic approximation to the lattice potential. In particular, a recent implementation of the quasi-harmonic approximation, in the Crystal program, is here shown to provide a reliable description of the thermal expansion coefficient, entropy, constant-volume and constant-pressure specific heats, and temperature dependence of the bulk modulus, nearly up to the corundum melting temperature. This is a remarkable outcome suggesting a-Al2O3 to be an almost

Received 16th March 2015, Accepted 1st April 2015

perfect quasi-harmonic crystal. The effect of using different computational parameters and DFT

DOI: 10.1039/c5cp01537e

functionals belonging to different levels of approximations on the accuracy of the thermal properties is tested, providing a reference for further studies involving alumina polymorphs and, more generally,

www.rsc.org/pccp

quasi-ionic minerals.

1 Introduction Aluminum oxide has been extensively used for decades in a wide variety of industrial applications due to its remarkable properties, including high melting point, density, electrical resistivity, hardness, resistance to weathering and low solubility.1 Corundum (a-Al2O3, the most stable form of aluminum oxide, whose atomic structure is sketched in Fig. 1) and its polymorphs (the so-called transitions aluminas) also exhibit unique surface properties, which make them suitable both as catalysts for several reactions2–9 and as supports for other catalysts.10–14 Furthermore, the thermodynamic properties of corundum are of particular interest in calorimetric studies in that it constitutes a standard reference material (SRM-720) for the calibration of some calorimeters.15 First-principles techniques based on the density functional theory (DFT) are becoming an important complementary tool in the investigation of mineral structure and thermodynamics, as well as surface properties and reactivity, as they allow us to

Fig. 1 Graphical representation of the atomic structure of corundum % (a-Al2O3, space group R3c): aluminum is colored in gray, oxygen in red. AlO6 octahedra and lattice parameters of the conventional cell are also represented.

a

Dipartimento di Chimica and Centre of Excellence Nanostructured Interfaces and ` di Torino, via Giuria 5, IT-10125 Torino, Italy. Surfaces (NIS), Universita E-mail: [email protected] b Laborato´rio de Combustı´veis e Materiais, INCTMN-UFPB, Universidade Federal da ˜o Pessoa, PB, Brazil Paraı´ba, CEP 58051-900, Joa c Nanochemistry Research Institute, Curtin Institute for Computation, and Department of Chemistry, Curtin University, GPO Box U1987, Perth, WA 6845, Australia

11670 | Phys. Chem. Chem. Phys., 2015, 17, 11670--11677

analyse the nature of the fundamental interactions giving rise to the observed phenomena.16 In this context, the ability to simulate realistic pressure and temperature conditions can make the diﬀerence between providing a qualitative or a quantitative prediction. In general, DFT modeling of solid state materials is performed at zero temperature and pressure, and

This journal is © the Owner Societies 2015

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

Paper

thermodynamic functions are estimated through harmonic lattice dynamics under the assumption of no thermal expansion. This is certainly a rough approximation, though successful in many cases and frequently used.17–21 However, this approach is unable to provide accurate predictions related to high temperature conditions, as well as to phases whose structures and properties have a significant dependence on temperature and pressure. Several computational studies on aluminum oxide polymorphs have been reported in recent years, which mainly apply standard DFT methods.22–30 In this paper, we apply a recently developed technique based on the so-called quasi-harmonic approximation (QHA): a simple and eﬀective method that is able to address the aforementioned issue in the case of corundum.31,32 The thermal expansion coeﬃcient, a(T), heat capacities, CV(T) and CP(T), entropy, S(T) and bulk modulus K(T) of corundum are calculated in their entire range of thermal stability (i.e. from 0 K up to its melting temperature, TM = 2317 K). The dependence of these properties on the level of approximation of the exchange–correlation functional, Vxc[r], is explicitly explored by considering six different expressions of Vxc[r], focusing on those ones that are widely adopted to calculate mineral properties (local density approximation, LDA; generalised gradient approximations, GGA; and hybrid functionals). The influence of other crucial computational parameters (e.g. supercell size in the calculation of phonon dispersion) on the calculated properties is also assessed. One of the main reasons of interest in the study of minerals simultaneously at high-temperatures and high-pressures is the characterization of their elastic response under geochemical Earth mantle conditions. Indeed, a necessary prerequisite to the understanding of how seismic waves do propagate during earthquakes is precisely the knowledge of the elastic response of all possible constituents of the Earth mantle. Conversely, the only source of information on the actual composition of the Earth mantle are seismic data collected during earthquakes; diﬀerent compositional models are used to interpret such data which strongly rely on the characterization of the elastic response of individual minerals under high temperature and pressure conditions.33–37 While a complete characterization of the thermoelasticity of a-Al2O3 would require the calculation of its fourth-rank elastic tensor at various temperatures and pressures (a quite demanding computational task which would give access to the full anisotropic description of the elastic response),38,39 the QHA offers a simplified approach to the investigation of the high-temperature, high-pressure behavior of an average elastic property of great geochemical interest: the bulk modulus K. Estimations of some thermal properties of corundum, based on Kieﬀer’s vibrational model with experimental frequency data, have been reported in the literature,40,41 as well as a couple of DFT studies where the QHA was applied to investigate phase transitions in alumina polymorphs.29,30,42 Mousavi has recently reported some quasi-harmonic thermal properties of corundum, as computed by a simplified Debye model (where the lattice dynamics of the crystal is not explicitly solved at the ab initio level of theory), which are found to largely disagree with available experimental data.43 To the best of our knowledge,

This journal is © the Owner Societies 2015

PCCP

the present investigation constitutes the first complete ab initio description of thermodynamic and thermal structural and elastic properties of a-Al2O3. This paper might then constitute a useful benchmark for undertaking future investigations involving aluminum oxide and related materials. The structure of the paper is as follows: in Section 2 we briefly recall the main features of the adopted implementation of the quasi-harmonic approximation and we introduce the utilized computational setup; results of the thermal eﬀects on structural and thermodynamic properties of a-Al2O3 are discussed in Section 3 where the eﬀect of the adopted functional of the DFT is explicitly investigated; the combined eﬀect of pressure and temperature on such properties is also quantified; conclusions are drawn in Section 4.

2 Computational approach and details All calculations are performed using a development version of the Crystal program,44,45 where a fully-automated scheme for computing quasi-harmonic properties of crystals has recently been implemented, which relies on computing and fitting harmonic vibration frequencies at diﬀerent volumes after having performed volume-constrained geometry optimizations.31,32 Such optimizations use analytical energy gradients with respect to both atomic coordinates and lattice parameters. Convergence is checked on energy, residual gradient components and magnitude of the nuclear displacements: default criteria are used.45 Harmonic phonon frequencies are computed by diagonalizing the dynamical matrix following a direct space approach. The influence of the adopted supercell size (equivalent to the sampling of the Brillouin zone in the reciprocal space approach) on the computed thermodynamic properties will be analyzed in Section 3. Further details about the ‘‘direct space’’ approach to phonon dispersion calculation can be found elsewhere.31,46–48 Constant-volume specific heat, CV(T), and entropy, S(T), are estimated through standard statistical thermodynamics from harmonic phonon frequencies as computed at the equilibrium zero temperature, and zero pressure volume. Other properties (such as the constant-pressure specific heat, the thermal expansion coeﬃcient or the temperature dependence of the bulk modulus), in order to be appropriately described, require to go beyond the simple harmonic approximation (HA) and are computed here by means of the QHA which is found to provide a satisfactory description of all of them nearly up to the melting temperature of corundum. The explored volume range extends from a 4.3% compression to a +8.6% expansion with respect to the equilibrium volume and four volumes are explicitly considered in this interval. The volumetric, isotropic, thermal expansion coeﬃcient, aV(T), is obtained by minimizing the isothermal Helmholtz free energy " !# hokp ðVÞ X k T QHA ZP B F ðT; VÞ ¼ U0 ðVÞ þ kB T ln 1 e ; (1) kp

with respect to volume at several temperatures, where kB is Boltzmann’s constant and UZP 0 (V) is the zero-temperature internal

Phys. Chem. Chem. Phys., 2015, 17, 11670--11677 | 11671

View Article Online

PCCP

Paper

energy of the crystal which includes the zero-point energy of the P system: E0ZP ðVÞ ¼ hokp ðVÞ 2. The scheme, recently developed

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

kp

and implemented into the Crystal program,31,32 is here generalized to the case of anisotropic thermal expansions: directional thermal expansion coeﬃcients, aa(T) and ac(T), corresponding to the a and c symmetry-independent lattice parameters of a-Al2O3 are computed, which allow for a finer description of the thermal expansion mechanism. One of the powerful advantages of the QHA is that of allowing for a natural combination of pressure and temperature eﬀects on structural and elastic properties of materials. By diﬀerentiating eqn (1) with respect to the volume and changing sign, the thermal pressure is obtained: PðV; TÞ ¼

@F QHA ðV; TÞ : @V

(2)

The description of the isothermal bulk modulus of the system at simultaneous high-temperatures and high-pressures, KT(P,T), can be obtained as an isothermal second derivative of eqn (1) with respect to the volume and by exploiting relation (2): 2 QHA @ F ðVðP; TÞ; TÞ KT ðP; TÞ ¼ VðP; TÞ : (3) @VðP; TÞ2 T

the system is suitably converged with respect to the sampling of the dispersion of phonon branches in reciprocal space. Equivalently, given the direct space nature of the approach utilized here, convergence of computed properties with the size of the adopted supercell (SC) has to be carefully checked for. If harmonic thermodynamic functions, such as entropy and constant-volume specific heat, show a rather slow convergence (more so for S than CV), the situation is generally much more favorable for quasi-harmonic ones. For instance, some of us have recently shown that for fully ionic systems, such as MgO and CaO, a SC containing 128 atoms is required to converge the entropy while a SC containing just 8 atoms already provides a converged description of all quasi-harmonic quantities.32 Fig. 2 shows such a convergence for entropy and constant-volume specific heat of a-Al2O3, as computed at the PBE0 level. Four SCs of increasing size are considered, containing 10, 30, 80 and 270 atoms and corresponding to the primitive cell, the conventional cell, a 2 2 2 expansion of the primitive cell and a 3 3 3 expansion of the primitive cell. It is seen that both quantities are practically converged with a SC containing 80 atoms, more so for CV than for S: at TM, the diﬀerences between

Let us finally recall that the QHA allows for computing the diﬀerence between constant-pressure and constant-volume specific heats as follows:49,50 CQHA CP(T) CV(T) = aV2(T)K(T)V(T)T.

(4)

All-electron atom-centered Gaussian-type-function basis sets, of TZVP quality, are adopted.51 Six diﬀerent formulations of the exchange–correlation functional of the DFT are considered, corresponding to some of the most widely used schemes within the LDA (SVWN52,53), GGA (PBE,54 PW91,55 PBEsol56) and hybrid approaches (B3LYP,57 PBE058). Thresholds controlling the accuracy of Coulomb and exchange series are set to 108 (T1 to T4) and 1016 (T5) for the integral truncation and to 1022 and 1018 for the selection of bi-electronic integrals that can be approximated by the bipolar expansion.45 Reciprocal space is sampled using a Monkhorst–Pack mesh with shrinking factors of 8, 4 and 2 when performing the calculation on the primitive cell, the conventional cell or largest cells (like a 2 2 2 or a 3 3 3 expansion of the primitive cell), corresponding to 65, 14 and 4 independent k-points in the irreducible portion of the Brillouin zone. A pruned grid with 1454 radial and 99 angular points is used to calculate the DFT exchange–correlation contribution through numerical integration of the electron density over the unit cell volume.45 The self-consistent-field (SCF) convergence on energy was set to a value of 1010 hartree for all geometry optimizations and phonon frequency calculations.

3 Results and discussion 3.1

Thermodynamic properties

When computing thermodynamic properties of crystals, one has to make sure that the description of the lattice dynamics of

11672 | Phys. Chem. Chem. Phys., 2015, 17, 11670--11677

Fig. 2 Specific heat, CV, (upper panel) and entropy S (lower panel) of a-Al2O3 as a function of temperature, as computed at the PBE0 level with SCs of increasing size: 10 (dots), 30 (dashed), 80 (dot-dashed) and 270 (continuous) atoms. The uppermost line of the top panel is the CP curve obtained by adding the CQHA quasi-harmonic contribution (evaluated according to eqn (4)) to the converged CV one. The inset of the upper panel shows the CV as computed using all the six DFT functionals considered in this study for the SC containing 30 atoms. Empty circles refer to experimental CV values from Saxena and Shen,59 full circles are experimental S and CP data from Robie et al.60

This journal is © the Owner Societies 2015

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

Paper

PCCP

the 80 and the 270 atom SCs are just 0.9% and 1.3% for CV and S, respectively. The SC containing 270 atoms is then expected to give results that are most likely to be fully converged. In the figure, we also report accurate experimental data to compare with: empty circles refer to CV values by Saxena and Shen59 while full circles to S values by Robie et al.60 For both quantities, the agreement between computed and experimental data is rather satisfactory in the whole temperature range and makes ab initio simulations a reliable predictive tool for these harmonic properties. Analogously to what recently documented for fully ionic systems,32 also in the present case of a mixed ionic–covalent system, the effect of the adopted DFT functional on such quantities is almost negligible as they both are dominated by acoustic modes generally correctly described by all functionals. In this respect, the inset of the upper panel of Fig. 2 shows CV as computed using the six DFT functionals considered in this study (LDA, PBE, PBEsol, PW91, B3LYP and PBE0) for the 30 atom SC; the six curves are essentially superimposed to each other. In the upper panel of the figure, the constant-pressure specific heat is also reported which will be commented on later as it is a quasiharmonic and not a simple harmonic quantity. The eﬀect of the SC size on the convergence of quasi-harmonic properties is shown in Fig. 3 where the diﬀerences between thermal expansion coeﬃcients, Da, and quasi-harmonic contribution to the specific heat, DCQHA, as computed with SCs of diﬀerent sizes and those obtained with the SC containing 80 atoms are reported. It is clearly seen that if the primitive cell (10 atoms) is not a suitable model, the conventional SC containing just 30 atoms provides a description of both quantities which are essentially converged, with an average deviation of 0.3% for CQHA and 0.9% for aV(T) over the whole temperature range with respect to the SC with 80 atoms. The eﬀect of the adopted DFT functional on the quasi-harmonic description will be discussed in Section 3.2. By adding the converged CQHA quasi-harmonic term to the converged CV harmonic contribution, the final constant-pressure

specific heat, CP, is obtained which is reported in the upper panel of Fig. 2 as a continuous line and compared with available experimental data by Robie et al.60 (full circles). This comparison shows how for a-Al2O3 the QHA is capable of correctly describing CP(T) up to its melting point, which is a remarkable result given that for most systems the validity domain of the QHA is restricted to temperatures well-below the melting one.32,61 This is a first evidence, to be further confirmed below, of the fact that a-Al2O3 corundum essentially behaves as an almost perfect quasiharmonic crystal, with no particular need for an explicit account of intrinsic anharmonic eﬀects beyond the QHA.

Fig. 3 Convergence of thermal expansion coeﬃcient aV(T) and CQHA (see eqn (4)) of a-Al2O3 as a function of the adopted SC size. Diﬀerences, Da and DCQHA, are reported with respect to the SC containing 80 atoms. All results are obtained using the PBE0 functional.

Fig. 4 Dependence of the conventional cell volume, V, and bulk modulus, K, of a-Al2O3 on temperature, as computed using diﬀerent DFT functionals at the quasi-harmonic level. Full and empty circles correspond to experimental data by Anderson et al.62 and Fiquet et al.,63 respectively.

This journal is © the Owner Societies 2015

3.2

Structural properties

The thermal behavior of structural and elastic properties of a-Al2O3 is now discussed as determined at the quasi-harmonic level of theory. The eﬀect on computed properties of the particular choice of the adopted DFT functional (three diﬀerent classes of functionals, LDA, GGA and hybrids, are explicitly considered) is discussed, which may serve as a benchmark for future studies on aluminum oxides. In Fig. 4, we report the equilibrium volume (of the conventional cell) and the bulk modulus of corundum as a function of temperature, up to its melting point. Experimental data are provided by Anderson et al.62 (full circles) and by Fiquet et al.63 (empty circles). From the analysis of the figure, some considerations can be made: (i) diﬀerent functionals do provide very diﬀerent values of the equilibrium volume and the bulk modulus, with diﬀerences

Phys. Chem. Chem. Phys., 2015, 17, 11670--11677 | 11673

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

PCCP

among them as large as 5% for the volume and 11% for the bulk modulus; (ii) as already observed in previous studies, the LDA functional provides the lowest volume and the highest bulk modulus among them while pure GGA functionals such as PBE and PW91 give the highest volumes and lowest bulk moduli; (iii) despite the very diﬀerent description of the absolute value of these properties, all functionals provide a fairly correct description of the temperature dependence of V and K almost up to TM, with small diﬀerences among them to be discussed below; (iv) surprisingly enough, in this case, the simple LDA functional provides results in excellent agreement with the experimental data, followed by the PBE0 hybrid functional; PBE and PW91, on the contrary, give the poorest description among those explored; (v) PBEsol, the PBE re-parametrization specifically designed for the solid state, significantly improves the description of both quantities, even if not to a suﬃcient extent to bring its results close to the experimental ones; (vi) the inclusion of the zero-point motion on zero-temperature values increases the volume by about 1% and decreases the bulk modulus by about 1.5% for all functionals (not shown in the figure). The exceptional performance of LDA in reproducing equilibrium structural features of a-Al2O3 has already been discussed in several ab initio studies.30,64–71 The good description of the temperature dependence of V(T) and K(T) up to TM, without strong deviations which are commonly seen in other systems (particularly on K(T)) well below TM,32 is a strong evidence of the quasi-harmonic character of a-Al2O3 corundum. Let us now analyze the description of the thermal expansion of a-Al2O3 in more detail. The upper panel of Fig. 5 shows the average isotropic thermal expansion coeﬃcient, a = aV/3, of corundum as computed using the six DFT functionals considered here. Accurate experimental data by Anderson et al.62 are reported as full circles. Despite an overall good description of the thermal expansion of corundum by all functionals, this figure allows for a finer discussion. It can be seen that three functionals (LDA, PBEsol and PBE0) perform better than the other three (PBE, PW91 and B3LYP) that slightly overestimate a. An interesting feature of the thermal expansion of non-cubic crystals is its anisotropy. If one considers the conventional cell of a-Al2O3, there are two symmetry-independent lattice parameters: a b and c; the corresponding directional thermal expansion coeﬃcients, aa(T) and ac(T), can be computed (the relation aV = 2aa + ac holds true). In the lower panel of Fig. 5 we report the ac aa diﬀerence as a function of temperature. Experimental data by Munro72 (full circles) and White and Roberts73 (empty circles) are also reported, the latter being not as smooth as the former ones. Some remarks can be made: (i) the ac aa diﬀerence is positive both experimentally and theoretically at all levels of theory thus implying a larger thermal expansion along the c crystallographic axis than in the basal plane ab; (ii) the anisotropy of the thermal expansion amounts to about 10% of the total; (iii) the steep behavior of experimental data by White and Roberts73 at temperatures below 250 K seems to be inconsistent with all theoretical predictions and other experimental data by Munro;72 (iv) the PBE0 hybrid functional describes an anisotropy which is very

11674 | Phys. Chem. Chem. Phys., 2015, 17, 11670--11677

Paper

Fig. 5 Mean isotropic ( a = aV/3) and anisotropic (ac aa) thermal expansion coeﬃcient of a-Al2O3 calculated as a function of temperature using various DFT functionals. Full circles represent experimental data by Anderson et al.62 for aV/3 and by Munro72 for ac aa; empty circles are data from White and Roberts.73

close to the experimental one by Munro,72 B3LYP provides a reasonable description up to about 600 K and then rapidly increases, while the other functionals seem to systematically overestimate it by about 20%. 3.3

Eﬀect of thermal pressure

While the inclusion of pressure on computed properties of solids can be considered a relatively simple task,37,77–82 the combined description of temperature and pressure is much more demanding and seldom reported in ab initio studies. As recalled in Section 2, one of the advantages of the quasiharmonic approximation is precisely that of allowing for a natural combination of both temperature and pressure on thermodynamic and structural properties of solids. The so-called thermal pressure can indeed be computed as a volume derivative of the isothermal Helmholtz free energy (see eqn (2)). The pressure– volume–temperature (P–V–T) equation-of-state (EOS) is then easily obtained. In Fig. 6, we report two different representations (which correspond to constant-pressure and constant-temperature experiments) of the P–V–T EOS of a-Al2O3, as computed using the hybrid PBE0 functional that has been found to reliably describe most of the properties discussed in the previous paragraphs. In the left panel of the figure, the V/V0 ratio (where V0 is the equilibrium volume at 300 K and zero pressure) is reported as a continuous function of temperature, up to corundum melting point, at five equidistant pressures (0, 3, 6, 9 and 12 GPa). Experimental data at

This journal is © the Owner Societies 2015

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

Paper

PCCP

Fig. 6 V/V0 as a function of temperature at 5 diﬀerent pressures (left panel) and as a function of pressure at 8 diﬀerent temperatures (right panel), where V0 is the equilibrium volume at 300 K and zero pressure of a-Al2O3. Full circles are experimental data from Anderson et al.62 (in the left panel) and from Sato and Akimoto74 (in the right panel), empty circles from Grevel et al.,75 while full squares and corresponding error bars are from Dubrovinsky et al.76 All computed values are obtained at the PBE0 level.

zero pressure by Anderson et al.62 are given as full circles while those at about 11 GPa by Dubrovinsky et al.76 as full squares, with corresponding error bars. The effect of pressure is a non-linear compression of the unit cell volume. The compression of the cell volume due to pressure is more pronounced at higher temperatures than at lower temperatures so that, as a result, pressure clearly reduces the thermal expansivity of a-Al2O3 (see below). In the right panel of the figure, we report the same quantity, V/V0, as a function of pressure at eight equidistant temperatures (0, 300, 600, 900, 1200, 1500, 1800 and 2100 K). Experimental data are also reported as measured at 300 K at different pressures by Sato and Akimoto74 (full circles), Grevel et al.75 (empty circles) and Dubrovinsky et al.76 (full square). We can clearly see that: (i) obviously as temperature increases the cell volume expands; (ii) a given volume (i.e. a given value of the V/V0 ratio) corresponds to higher pressures as temperature increases. As we have just anticipated, from the inspection of the left panel of Fig. 6 one can see how pressure is progressively reducing the thermal expansivity of corundum. In order to give a more quantitative representation of such eﬀect we introduce the upper panel of Fig. 7 where the volumetric thermal expansion coeﬃcient, aV, of a-Al2O3 is plotted as a function of temperature at five equidistant pressures. Experimental data at zero pressure, from Anderson et al.,62 are in excellent agreement with PBE0 theoretical ones, as already noticed while discussing Fig. 5. It is clearly seen that, as pressure linearly increases, the thermal expansivity of corundum decreases (not linearly). As we could not find any high-pressure experimental data of the thermal expansion coeﬃcient of a-Al2O3 and given the excellent description provided by the hybrid PBE0 functional so far, these values are expected to constitute reliable predictions of the hightemperature, high-pressure behavior of corundum. As recalled in the Introduction, the description of the bulk modulus of minerals simultaneously under high temperature and pressure conditions is of particular geochemical interest. In the lower panel of Fig. 7, we report the isothermal bulk modulus, KT, computed as the volume second derivative of the

This journal is © the Owner Societies 2015

Fig. 7 Dependence on temperature, up to 2300 K, and pressure, up to 12 GPa, of the thermal expansion coeﬃcient (upper panel) and bulk modulus (lower panel) of a-Al2O3, as computed at the PBE0 level. Experimental data at ambient pressure from Anderson et al.62 are reported for comparison. In the lower panel, full circles refer to the isothermal bulk modulus, KT, while empty circles to the adiabatic bulk modulus, KS. In the lower panel, the dashed line represents the computed adiabatic bulk modulus at zero pressure.

isothermal Helmholtz free energy (see eqn (3)). It is reported as a continuous function of temperature at five distinct pressures, up to 12 GPa. Pressure is seen to systematically increase the bulk modulus, more so at higher temperatures. Isothermal experimental determinations at zero pressure from Anderson et al.62 are reported as full circles. The agreement with the PBE0 theoretical description (lowest continuous line) is remarkable in the whole temperature range. Some experimental techniques for measuring the bulk modulus of a crystal involve elastic waves and are characterized by very short time-scales that prevent the system from reaching a thermal equilibrium; in these cases, an adiabatic bulk modulus, KS, is measured. Adiabatic and isothermal bulk moduli do coincide with each other at zero temperature only, with KS always being larger than KT at any finite temperature. In the figure, for instance, empty circles do represent adiabatic bulk modulus values as measured at zero pressure by Goto et al.83 with the rectangular parallelepiped resonance method. The QHA also oﬀers a way to compute the adiabatic bulk modulus from the isothermal one, given that

KS ¼ KT þ

aV 2 VTKT 2 CP ¼ KT ; CV CV

(5)

Phys. Chem. Chem. Phys., 2015, 17, 11670--11677 | 11675

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

PCCP

where the dependence of all quantities on temperature is omitted for clarity sake and in the last equality eqn (4) has been exploited. The computed adiabatic bulk modulus at zero pressure is reported in the figure as a dashed line; again, the agreement with the experimental determinations is quite remarkable and confirms once more how the QHA allows for accurately describing structural and elastic features of a-Al2O3 up to the melting temperature.

4 Conclusions The dependence of a variety of thermodynamic, structural and elastic properties of a-Al2O3 on temperature has been accurately determined by means of ab initio simulations exploiting both the harmonic and quasi-harmonic approximations. The validity domain of the quasi-harmonic approximation, being often limited to temperatures much lower than the melting point TM, is here found to extend almost up to TM thus suggesting that corundum essentially behaves as a perfect quasi-harmonic crystal with negligible intrinsic anharmonic eﬀects. As other aluminum oxide polymorphs exhibit analogous structural and chemical features, from present results, the quasi-harmonic approximation is expected to constitute an eﬀective and reliable approach to their thermal characterization. The eﬀect of the adopted functional of the density functional theory on thermal properties of a-Al2O3 has been explicitly investigated and will prove a useful benchmark for future theoretical studies requiring a good thermodynamic description of aluminum oxides. Six diﬀerent formulations, belonging to three diﬀerent rungs of the ‘‘Jacob’s ladder’’, have been considered: (i) all functionals accurately describe harmonic thermodynamic properties such as entropy and constant-volume specific heats; (ii) the simple LDA functional fortuitously provides an excellent description of the absolute values of both cell volume and bulk modulus of corundum; (iii) all functionals are seen to correctly describe isotropic thermal properties up to TM; (iv) the hybrid PBE0 functional gives the best description of the thermal expansion coeﬃcient (including its anisotropy which is overestimated by about 20% by the other functionals). The combined eﬀect of temperature and pressure, up to 12 GPa, has been predicted for structural and elastic properties, which has a particular relevance to the field of geochemistry where such characterizations are extremely useful in finetuning and validating diﬀerent compositional models for the Earth mantle.

Acknowledgements ˆncia J.M. acknowledges the Brazilian scholarship program ‘‘Cie sem Fronteiras’’ (Process Number 248425/2013-7/SWE). RDe acknowledges Curtin University for funding through the Curtin Research Fellowship scheme, iVEC facilities and the Australian National Computing Infrastructure for the provision of computer time.

11676 | Phys. Chem. Chem. Phys., 2015, 17, 11670--11677

Paper

References 1 L. D. Hart, Alumina Chemicals: Science And Technology Handbook, The American Ceramic Society, Westerville, Ohio, 1990. ¨ck, Ø. Borck, E. Schro ¨der and B. I. Lundqvist, 2 S. D. Chakarova-Ka Phys. Rev. B: Condens. Matter Mater. Phys., 2006, 74, 155402. ¨der, Phys. Rev. B: Condens. 3 Ø. Borck, P. Hyldgaard and E. Schro Matter Mater. Phys., 2007, 75, 035403. 4 V. A. Ranea, I. Carmichael and W. F. Schneider, J. Phys. Chem. C, 2009, 113, 2149. 5 Y. Zhao, Z. Chen and J. Zhao, Environ. Sci. Technol., 2010, 44, 2035. 6 J. G. Catalano, J. Phys. Chem. C, 2010, 114, 6624. 7 D. P. Woodruﬀ, Chem. Rev., 2013, 113, 3863. 8 J. H. Park, K. Kim, Y. B. Yoo, S. Y. Park, K.-H. Lim, K. H. Lee, H. K. Baik and Y. S. Kim, J. Mater. Chem. C, 2013, 1, 7166. 9 M. Ruan, H. Hou, W. Li and B. Wang, J. Phys. Chem. C, 2014, 118, 20889. 10 T. J. Godin and J. P. LaFemina, Phys. Rev. B: Condens. Matter Mater. Phys., 1994, 49, 7691. 11 P. Bera, K. C. Patil, V. Jayaram, M. S. Hegde and G. N. Subbanna, J. Mater. Chem., 1999, 9, 1801. 12 T. K. Todorova, M. V. Ganduglia-Pirovano and J. Sauer, J. Phys. Chem. C, 2007, 111, 5141. ¨nbeck, J. Phys. Chem. C, 2009, 113, 3674. 13 A. Hellman and H. Gro 14 J. L. Achtyl, I. V. Vlassiouk, S. Dai and F. Geiger, J. Phys. Chem. C, 2014, 118, 17745. 15 D. G. Archer, J. Phys. Chem. Ref. Data, 1993, 22, 1441. 16 G. E. Brown, Jr and G. Calas, Mineral-Acqueous Solution Interfaces and Their Impact on the Environment (European Association of Geochemistry, 2012–2013), vol. 1(6) of Geochemical Perspectives, ch. 6, pp. 540–544. 17 R. Demichelis, P. Raiteri, J. D. Gale and R. Dovesi, J. Phys. Chem. C, 2013, 117, 17814. ˜ oz-Garcı´a, M. Pavone, J. A. Keith 18 A. M. Ritzmann, A. B. Mun and E. A. Carter, Chem. Mater., 2013, 25, 3011. 19 M. Digne, P. Sautet, P. Raybaud, P. Euzen and H. Toulhoat, J. Catal., 2002, 211, 1. 20 C. Wolverton and K. C. Hass, Phys. Rev. B: Condens. Matter Mater. Phys., 2001, 63, 024102. ¨l, P. Ugliengo, C. M. Zicovich-Wilson 21 R. Demichelis, Y. Noe and R. Dovesi, J. Phys. Chem. C, 2011, 115, 13107. 22 M. F. Peintinger, M. J. Kratz and T. Bredow, J. Mater. Chem. A, 2014, 2, 13143. 23 J. Sarsam, M. W. Finnis and P. Tangney, J. Chem. Phys., 2013, 139, 204704. 24 C. K. Narula and G. M. Stocks, J. Phys. Chem. C, 2012, 116, 5628. 25 S. Aryal, P. Rulis, L. Ouyang and W. Y. Ching, Phys. Rev. B: Condens. Matter Mater. Phys., 2011, 84, 174123. ˜o and S. de ¨kbenli, A. A. Leita ¨c¸u 26 A. R. Ferreira, E. Ku Gironcoli, Phys. Rev. B: Condens. Matter Mater. Phys., 2011, 84, 235119. 27 B. Xu, H. Stokes and J. Dong, J. Phys.: Condens. Matter, 2010, 22, 315403. 28 K. Jiang, D. Music, K. Sarakinos and J. Schneider, J. Phys.: Condens. Matter, 2010, 22, 505502.

This journal is © the Owner Societies 2015

View Article Online

Published on 01 April 2015. Downloaded by Nanyang Technological University on 20/05/2015 10:01:05.

Paper

29 K. Umemoto and R. M. Wentzcovitch, Proc. Natl. Acad. Sci. U. S. A., 2008, 105, 6526. 30 A. R. Oganov and S. Ono, Proc. Natl. Acad. Sci. U. S. A., 2005, 102, 10828. 31 A. Erba, J. Chem. Phys., 2014, 141, 124115. 32 A. Erba, M. Shahrokhi, R. Moradian and R. Dovesi, J. Chem. Phys., 2015, 142, 044114. 33 A. E. Ringwood, Composition and Petrology of the Earth’s Mantle, McGraw-Hill, New York, 1975. 34 J. D. Bass and D. L. Anderson, Geophys. Res. Lett., 1984, 11, 229. 35 D. L. Anderson and J. D. Bass, Nature, 1986, 320, 321. 36 A. Erba, A. Mahmoud, R. Orlando and R. Dovesi, Phys. Chem. Miner., 2014, 41, 151. 37 A. Erba, A. Mahmoud, D. Belmonte and R. Dovesi, J. Chem. Phys., 2014, 140, 124703. 38 B. B. Karki, R. M. Wentzcovitch, S. de Gironcoli and S. Baroni, Science, 1999, 286, 1705. 39 B. B. Karki, R. M. Wentzcovitch, S. de Gironcoli and S. Baroni, Phys. Rev. B: Condens. Matter Mater. Phys., 2000, 61, 8793. 40 P. F. McMillan and N. L. Ross, Phys. Chem. Miner., 1987, 14, 225. 41 J.-A. Xu, E. Huang, J.-F. Lin and L. Y. Xu, Am. Mineral., 1995, 80, 1157. ´ ski, Phys. Rev. B: Condens. Matter 42 Z. Łodziana and K. Parlin Mater. Phys., 2003, 67, 174106. 43 S. Mousavi, J. Optoelectron. Adv. Mater., 2014, 8, 1191. 44 R. Dovesi, R. Orlando, A. Erba, C. M. Zicovich-Wilson, B. Civalleri, S. Casassa, L. Maschio, M. Ferrabone, M. De La Pierre and Ph. D’Arco, et al., Int. J. Quantum Chem., 2014, 114, 1287. 45 R. Dovesi, V. R. Saunders, C. Roetti, R. Orlando, C. M. Zicovich-Wilson, F. Pascale, K. Doll, N. M. Harrison, B. Civalleri and I. J. Bush, et al., CRYSTAL14 User’s Manual, ` di Torino, Torino, 2014, http://www.crystal.unito.it. Universita 46 A. Erba, M. Ferrabone, R. Orlando and R. Dovesi, J. Comput. Chem., 2013, 34, 346. 47 K. Parlinski, Z. Q. Li and Y. Kawazoe, Phys. Rev. Lett., 1997, 78, 4063. 48 A. Togo, F. Oba and I. Tanaka, Phys. Rev. B: Condens. Matter Mater. Phys., 2008, 78, 134106. 49 R. E. Allen and F. W. De Wette, Phys. Rev., 1969, 179, 873. 50 L. L. Boyer, Phys. Rev. Lett., 1979, 42, 584. 51 M. F. Peintinger, D. V. Oliveira and T. Bredow, J. Comput. Chem., 2013, 34, 451. 52 J. C. Slater, Phys. Rev., 1951, 81, 385. 53 S. H. Vosko, L. Wilk and M. Nusair, Can. J. Phys., 1980, 58, 1200. 54 J. P. Perdew, K. Burke and M. Ernzerhof, Phys. Rev. Lett., 1996, 77, 3865. 55 J. Perdew, J. Chevary, S. Vosko, K. Jackson, M. Pederson, D. Singh and C. Fiolhais, Phys. Rev. B: Condens. Matter Mater. Phys., 1992, 46, 6671.

This journal is © the Owner Societies 2015

PCCP

56 J. Perdew, A. Ruzsinsky, G. I. Csonka, O. A. Vydrov, G. E. Scuseria, L. A. Constantin, X. Zhou and K. Burke, Phys. Rev. Lett., 2008, 100, 136406. 57 A. D. Becke, J. Chem. Phys., 1993, 98, 5648. 58 C. Adamo and V. Barone, J. Chem. Phys., 1999, 110, 6158. 59 S. K. Saxena and G. Shen, J. Geophys. Res., B, 1992, 97, 19813. 60 R. A. Robie, B. S. Hemingway and J. R. Fisher, Tech. Rep. B-1452, United States Geological Survey, 1978. 61 B. B. Karki and R. M. Wentzcovitch, Phys. Rev. B: Condens. Matter Mater. Phys., 2003, 68, 224304. 62 O. L. Anderson, D. L. Isaak and H. Oda, J. Geophys. Res., B, 1991, 96, 18037. 63 G. Fiquet, P. Richet and G. Montagnac, Phys. Chem. Miner., 1999, 27, 103. 64 F. C. Marton and R. E. Cohen, Am. Mineral., 1994, 79, 789. 65 W. Duan, B. B. Karki and R. M. Wentzcovitch, Am. Mineral., 1999, 84, 1961. 66 R. Caracas and R. E. Cohen, Geophys. Res. Lett., 2005, 32, L06303. 67 B. Montanari, B. Civalleri, C. M. Zicovich-Wilson and R. Dovesi, Int. J. Quantum Chem., 2006, 106, 1703. 68 M. Iuga, G. Steinle-Neumann and J. Meinhardt, Eur. Phys. J. B, 2007, 58, 127. 69 K. Kunc and K. Syassen, Phys. Rev. B: Condens. Matter Mater. Phys., 2010, 81, 134102. 70 D. P. Sigumonrong, D. Musici and J. M. Schneider, Comput. Mater. Sci., 2011, 50, 1197. 71 A. Dewaele and M. Torrent, Phys. Rev. B: Condens. Matter Mater. Phys., 2013, 88, 064107. 72 R. G. Munro, J. Am. Ceram. Soc., 1997, 80, 1919. 73 G. K. White and R. B. Roberts, High Temp. – High Pressures, 1983, 15, 321. 74 Y. Sato and S. Akimoto, J. Appl. Phys., 1979, 50, 5285. 75 K.-D. Grevel, M. Burchard, D. W. Fahauer and T. Peun, J. Geophys. Res., 2000, 105, 27877. 76 L. S. Dubrovinsky, S. K. Saxena and P. Lazor, Phys. Chem. Miner., 1998, 25, 434. 77 A. Mahmoud, A. Erba, K. Doll and R. Dovesi, J. Chem. Phys., 2014, 140, 234703. 78 A. Erba, L. Maschio, S. Salustro and S. Casassa, J. Chem. Phys., 2011, 134, 074502. 79 A. Erba, L. Maschio, C. Pisani and S. Casassa, Phys. Rev. B: Condens. Matter Mater. Phys., 2011, 84, 012101. 80 V. Lacivita, A. Erba, R. Dovesi and Ph. D’Arco, Phys. Chem. Chem. Phys., 2014, 16, 15331. ´pez, V. Lacivita, P. D’Arco and 81 A. Erba, A. M. Navarrete-Lo C. M. Zicovich-Wilson, Phys. Chem. Chem. Phys., 2015, 17, 2660. 82 J. Maul, A. Erba, I. M. G. Santos, J. R. Sambrano and R. Dovesi, J. Chem. Phys., 2015, 142, 014505. 83 T. Goto, O. L. Anderson, I. Ohno and S. Yamamoto, J. Geophys. Res., B, 1989, 94, 7588.

Phys. Chem. Chem. Phys., 2015, 17, 11670--11677 | 11677